# Presentation: 683502

## Dale P. Bentz (dale.bentz@nist.gov)
National Institute of Standards and Technology
Prepared for: Mid-Atlantic Region Quality Assurance Workshop
February 2006

- National Institute of Standards and Technology
- Prepared for: Mid-Atlantic Region Quality Assurance Workshop
- February 2006

- Internal Curing - Questions and Answers

## Collaborators

- NIST - Mr. Max Peltz and Dr. Kenneth A. Snyder
- Mr. Thomas A. Holm (ESCSI)
- Mr. John W. Roberts (Northeast Solite)
- Pennsylvania State University
- Profs. Phillip M. Halleck and Abraham S. Grader
- Technical University of Denmark
- Profs. Mette Geiker, Ole M. Jensen, and Pietro Lura

## Question: What is internal curing (IC)?

Answer: As being considered by ACI-308, “internal curing refers to the process by which the hydration of cement occurs because of the availability of additional internal water that is not part of the mixing water.”

For many years, we have been curing concrete from the outside in, internal curing is for curing from the inside out.  Internal water is generally supplied via internal reservoirs, such as saturated lightweight fine aggregates, superabsorbent  polymers, or saturated wood fibers.

- Answer: ***As being considered by ACI-308, “internal curing refers to the process by which the hydration of cement occurs because of the availability of additional ***_***internal***_*** water that is not part of the mixing water.”***
- For many years, we have been curing concrete from the outside in, internal curing is for curing from the inside out.  Internal water is generally supplied via internal reservoirs, such as ***saturated*** lightweight fine aggregates, superabsorbent  polymers, or ***saturated*** wood fibers.

## Question: What are the problems in pavements that IC can address?
Answer: While internal curing offers many potential benefits, for pavements, the major problem that it may alleviate is CRACKING!
2003 FHWA Nationwide HPC Survey Results --- Most Common Pavement Distresses
	1) Early-age deck cracking (56.6 % of responses were a 4 or 5=often)
	2) Corrosion (42.3 % ---- definitely linked to cracking)
	3) Cracking of girders, etc. (31.4 %)
	Others (sulfate attack, ASR, F/T, overload, poor construction quality were all below 25 % level)

- Answer: ***While internal curing offers many potential benefits, for pavements, the major problem that it may alleviate is CRACKING!***
- 2003 FHWA Nationwide HPC Survey Results --- Most Common Pavement Distresses
- 	1) Early-age deck cracking (56.6 % of responses were a 4 or 5=often)
- 	2) Corrosion (42.3 % ---- definitely linked to cracking)
- 	3) Cracking of girders, etc. (31.4 %)
- 	Others (sulfate attack, ASR, F/T, overload, poor construction quality were all below 25 % level)

## Early-Age Cracking Contributors

**Thermal Effects**
- Hydration heat can raise concrete temperature significantly (causing expansion), subsequent thermal contraction during cooling can lead to early-age (global or local) cracking if restrained (globally or locally)
**Autogenous Shrinkage**
- In lower w/cm concretes, if sufficient curing water can not be supplied externally, the ***chemical shrinkage*** that accompanies the hydration reactions will lead to ***self-desiccation*** and significant ***autogenous shrinkage*** (and possibly cracking)

## Some Terminology(from RILEM ICC committee)

**Chemical shrinkage**
- An internal volume reduction that is the result of the fact that the absolute volume of the hydration products is less than that of the reactants (cement and water); can be on the order of 10 % by volume; new ASTM standard test method is C1608
**Self-desiccation **
- The reduction in the internal relative humidity (RH) of a sealed system when empty pores are generated.
**Autogenous shrinkage**
- The external (macroscopic) dimensional reduction of the cementitious system under isothermal, sealed curing conditions; can be 100 to 1000 microstrains

## Example of Chemical Shrinkage (CS)

- Hydration of tricalcium silicate
- C3S + 5.3 H  C1.7SH4 + 1.3 CH
- Molar volumes
- 			71.1 + 95.8  107.8 + 43
- CS = (150.8 – 166.9) / 166.9 = -0.096 mL/mL or
- 	-0.0704 mL/g cement
- For each lb (g) of tricalcium silicate that reacts completely, we need to supply 0.07 lb (g) of *extra* curing water to maintain saturated conditions (In 1935, Powers measured a value of 0.053 for 28 d hydration – 75 %)

## From Chemical Shrinkage to Autogenous Shrinkage

- CS creates empty pores within
- 		hydrating paste
- During self-desiccation, internal RH and capillary stresses are both regulated by the size of the empty pores being created
- These stresses result in a physical autogenous deformation (shrinkage strain) of the specimen
- Analogous to drying shrinkage, but drying is internal.

## Question: Why do we need IC?

Answer: Particularly in HPC, it is not easily possible to provide curing water from the top surface (for example) at the rate that is required to satisfy the ongoing chemical shrinkage, due to the extremely low permeabilities that are often achieved in the concrete as the capillary pores depercolate.
Capillary pore percolation/depercolation first noted by Powers, Copeland and Mann (PCA-1959).

- Answer: ***Particularly in HPC, it is not easily possible to provide curing water from the top surface (for example) at the rate that is required to satisfy the ongoing chemical shrinkage, due to the extremely low permeabilities that are often achieved in the concrete as the capillary pores depercolate.***
***Capillary pore percolation/depercolation first noted by Powers, Copeland and Mann (PCA-1959).***

## Question: How does IC work?

Answer: IC distributes the extra curing water throughout the 3-D concrete microstructure so that it is more readily available to maintain saturation of the cement paste during hydration, avoiding self-desiccation (in the paste) and reducing autogenous shrinkage.
Because the autogenous stresses are inversely proportional to the diameter of the pores being emptied, for IC to do its job, the individual pores in the internal reservoirs should be much larger than the typical sizes of the capillary pores (micrometers) in hydrating cement paste.

- Answer: ***IC distributes the extra curing water throughout the 3-D concrete microstructure so that it is more readily available to maintain saturation of the cement paste during hydration, avoiding self-desiccation (in the paste) and reducing autogenous shrinkage.***
- Because the autogenous stresses are inversely proportional to the diameter of the pores being emptied, for IC to do its job, the individual pores in the internal reservoirs should be much larger than the typical sizes of the capillary pores (micrometers) in hydrating cement paste.

## Cement 

***Cement ***
***paste***

**Water reservoir**

## Question: How can the effectiveness of IC be quantified?
Answer: By direct and indirect experimental measurements including –
		internal RH
		autogenous deformation
		compressive strength development
		degree of hydration
		restrained shrinkage or ring tests
		3-D X-ray microtomography

- Answer: ***By direct and indirect experimental measurements including –***
***	******	******internal RH***
***	******	******autogenous deformation***
***	******	******compressive strength development***
***	******	******degree of hydration***
***	******	******restrained shrinkage or ring tests***
***	******	******3-D X-ray microtomography***

## Internal RH, How to measure it? 

- On small volumes of mortar in sealed containers using Rotronic Hygroscope DT RH stations (at
- 	Technical University of Denmark)

**Grasley, Lange, and D’Ambrosia at UIUC have recently developed **
**a small insitu temperature/RH sensor for use in (field) concrete**

## Internal RH ResultsMortars with Internal CuringLWA = saturated lightweight aggregatesSAP = superabsorbent polymerFSF = control with fine silica fume

**w/cm = 0.35**

## Autogenous Deformation, How to measure it?  

- One way is with custom-built digital dilatometers *(O.M. Jensen - DTU)*
- Specimens sealed in corrugated polymer tubes and stored at
-    constant
-    temperature

**Method under consideration for standardization by ASTM C09.68**

## Autogenous Deformation Results

**w/cm = 0.35**

## Degree of Hydration and Strength

**w/cm = 0.35**

## Three-Dimensional X-ray Microtomography

- X-ray microtomography allows direct observation of the 3-D microstructure of cement-based materials
- Example: Visible Cement Data Set _[http://visiblecement.nist.gov](http://visiblecement.nist.gov/)_
- In October 2005, experiments were conducted at Pennsylvania State University to monitor three-dimensional water movement during internal curing of a high-performance mortar over the course of two days

## After mixing

**After mixing**

**1 d hydration**

**2 d hydration**

**Subtraction: 1 d – after mixing**

**Aqua indicates drying**
**Red indicates wetting**

- All images are 13 mm
- 	by 13 mm

## Three-Dimensional X-ray Microtomography

**Three-dimensional subtracted image**
**of 1 d hydration – initial microstructure**
**showing water-filled pores that have **
**emptied during internal curing **
**(4.6 mm on a side)**

**2-D image with water evacuated**
**regions (pores) overlaid on **
**original microstructure**
**(4.6 mm by 4.6 mm)**

_**Three-Dimensional X-ray Microtomography**_

## Questions to Consider When Using IC

- How much water (or LWA) do I need to supply for internal curing?
- How far can the water travel from the surfaces of the internal reservoirs?
- How are the internal reservoirs distributed within the 3-D concrete microstructure?
- Answers
- 	May be found at the NIST internal curing web site: _[http://ciks.cbt.nist.gov/lwagg.html](http://ciks.cbt.nist.gov/lwagg.html)_

## http://ciks.cbt.nist.gov/lwagg.html

**Menu for Internal Curing with Lightweight Aggregates**
**1)**_[Calculate Lightweight Aggregates Needed for Internal Curing](http://ciks.cbt.nist.gov/~bentz/lwavolume.html)_
** **
**2)**_[Estimation of Travel Distance of Internal Curing Water](http://ciks.cbt.nist.gov/~bentz/water_distance.html)__ _
**3)**_[Simulate Mixture Proportions to View Water Availability Distribution](http://ciks.cbt.nist.gov/~bentz/intcuring.html)_
** **
**4)**_[View Water Availability Distribution Simulation Results](http://ciks.cbt.nist.gov/~bentz/icresults.html)__ _
**5)**_[Learn more about FLAIR: Fine Lightweight Aggregates as Internal Reservoirs for the autogenous distribution of chemical admixtures](http://ciks.cbt.nist.gov/~bentz/flairintro.html)_

## Question: How much water (or LWA) do I 	need to supply for internal curing?

- Answer: ***Equation for mixture proportioning***
***	******	***(Menu selection #1)
*M*LWA =mass of (dry) LWA needed per unit volume of concrete
*C**f* =cement factor (content) for concrete mixture
*CS* =(measured via ASTM C 1608-05 or computed) chemical shrinkage of cement
- α*max* =maximum expected degree of hydration of cement, [(w/c)/0.36] or 1
*S* =degree of saturation of LWA (0 to 1] when added to mixture
- øLWA = (measured) absorption of lightweight aggregate (use desorption measured at 93 % RH (potassium nitrate saturated salt solution) via ASTM C 1498–04a)

## Question: How far can the water travel from the surfaces of the LWA?

- Answer: ***Equation balancing water needed (hydration) vs. water available (flow) ******	***(Menu selection #2)
***	***“Reasonable” estimates ---
- 		early hydration ---- 20 mm
- 		middle hydration --- 5 mm
- 		late hydration --- 1 mm or less
- 		“worst case” --- 0.25 mm (250 μm)
- Early and middle hydration estimates in agreement with x-ray absorption-based observations on mortars during curing

## Question: How are the internal reservoirs 	distributed within the 3-D concrete 	microstructure?

- Answer: ***Simulation using NIST Hard Core/Soft Shell (HCSS) Computer Model ***(Menu selections #3 and #4)
- Returns a table of “protected paste
- fraction” as a function of distance
- from LWA surface

- Yellow – Saturated LWA
- Red – Normal weight sand
- Blues – Pastes within various
- 	distances of an LWA

**10 mm by 10 mm**

## Question: What does the future hold?

Answer: 
	- Likely that some more state DOTs will   
		begin to evaluate internal curing
	- Investigation of possible “air void” system
		provided by empty internal reservoirs
	- Usage of internal reservoirs to distribute 	chemical admixtures as well as water (SRAs, 	corrosion inhibitors, ASR mitigation admixtures)
		FLAIR – Fine Lightweight Aggregates as 			Internal Reservoirs 
(Menu selection #5 on NIST internal curing web site; 
being investigated by W.R. Grace, Sika, and Maxit)

- Answer:
- 	- ***Likely that some more state DOTs will   ***
***	******	******begin to evaluate internal curing***
***	******-****** Investigation of possible “air void” system***
***	******	******provided by empty internal reservoirs***
***	******-****** Usage of internal reservoirs to distribute ******	******chemical admixtures as well as water ******(SRAs, ******	******corrosion inhibitors, ASR mitigation admixtures)***
***	******	******FLAIR – Fine Lightweight Aggregates as ******	******	******	******Internal Reservoirs ***
***(Menu selection #5 on NIST internal curing web site; ***
***being investigated by W.R. Grace, Sika, and Maxit)***

## Question: Who (else) is active in this area of research/application?
Answer: 
	- NIST
	- NRC/Canada (Dr. Daniel Cusson)
	- Cleveland State University (Prof. Delatte for Ohio DOT)
	- RILEM-ICC (Dr. Kosta Kovler – Technion, Israel)
	- Georgia Tech University (Profs. Mohr and Kurtis)
	- Technical University of Denmark (Prof. Ole Jensen and Dr. Pietro Lura – superabsorbent polymers)
	- University of Toronto (Prof. Hooton and Hoa Lam)
	- TXI (job in Texas, spring 2005 – 238,000 yd3 concrete)
	- U.S. Concrete (specified density concrete)

- Answer:
- 	- ***NIST***
***	******- ******NRC/Canada ******(Dr. Daniel Cusson)***
- 	- ***Cleveland State University ******(Prof. Delatte for Ohio DOT)***
- 	- ***RILEM-ICC ******(Dr. Kosta Kovler – Technion, Israel)***
- 	- ***Georgia Tech University ******(Profs. Mohr and Kurtis)***
***	******- ******Technical University of Denmark ******(Prof. Ole Jensen and Dr. Pietro Lura – superabsorbent polymers)***
***	******-****** ******University of Toronto (Prof. Hooton and Hoa Lam)***
***	******- ******TXI (job in Texas, spring 2005 – 238,000 yd******3****** concrete)***
***	******-****** U.S. Concrete (specified density concrete)***

## Thank you !More Questions ????